ALUMINIUM – FLY ASH COMPOSITES AS LIGHT WEIGHT
MATERIALS FOR AUTOMOTIVE INDUSTRY
Department of Mechanical Engineering, Karpagam College of Engineering, Coimbatore-641032.
Department of Metallurgy, PSG College of Technology, Coimbatore-641004
Department of Automobile Engineering, Karpagam University, Coimbatore-641021
Development of lightweight materials has provided the
automotive industry with numerous possibilities for
vehicle weight reduction. Progress in this area depends
on the development of metallurgy, casting and
solidification techniques, heat and surface treatments.
Since fuel consumption relates directly to vehicle weight,
reducing weight can improve the fuel usage and price-toperformance
Aluminium matrix ceramic reinforcement composites
have attracted more attention due to their combined
properties such as high specific strength, high stiffness,
low thermal expansion coefficient and superior
dimensional stability at elevated temperatures as
compared to the monolithic materials. Aluminium
reinforced with conventional ceramic materials such as
SiC / Al2O3 are gradually being implemented into the
production of pistons, cylinders, engine blocks, brakes
and power transfer system elements in automobile
Fly ash (SiO2, Al2O3, Fe2O3 as major constituents and
oxides of Mg, Ca, Na, K etc. as minor constituents) is
one of the most inexpensive and low density material
which is abundantly available as solid waste byproduct
during combustion of coal in thermal power plants.
The present investigation has been focused on the
utilization of fly ash in useful manner by dispersing it into
aluminium to produce composites by two step stir
casting method to over come the cost barrier for wide
spread applications in automotive systems. Also an
attempt has been made to investigate its microstructure,
mechanical, wear and corrosion behavior of composites.
Keywords: Aluminium matrix composites; fly ash; two
step stir casting
Metal matrix composites (MMCs), particularly aluminium
matrix ceramic reinforcement composites have emerged
as a potential material especially for automotive and
In this study, fly ash particles which are extracted from
residues generated in the combustion of coal were
chosen as reinforcement material. India produces about
110 million tons of fly ash per year from burning about
250 million tons of coal for electric power generation.
Apart from energy and cost savings, green house gases
that are generated during the production of Al may be
significantly reduced by decreasing the production of Al
by fly ash substitution. Limited attempts have been made
in investigating the effect of fly ash on aluminium matrix.
Among various processing techniques, stir casting
appears to be most promising route for production of
aluminium matrix composites because of simplicity and
able to produce the composites in large scale
In any production process, superior quality of the product
can be achieved only while the process is run with the
optimum parameters. Mechanical properties of
composites are affected by the size and shape of the
matrix and reinforcement materials, weight fraction of the
reinforcement and reaction at the interface. The
reinforcement plays a significant role in determining the
properties of MMCs. These aspects have been
discussed by many researchers.
Fly ash particles were incorporated into the molten Al
they were observed to be floating on the molten Al
surface due to the high surface tension which leads poor
Since the gas layers at the surfaces of the particles can
cause the buoyant migration, mechanical stirring can be
done in a semi solid state rather than in the completely
liquid state in order to break away the gas layers thereby
reducing surface tension.
Wettability can be improved by increasing the surface
energies of the solids, decreasing the surface tension of
the liquid matrix alloy and decreasing the solid/liquid
interfacial energy at the reinforcement matrix interface.
The magnesium which acts as a powerful surfactant as
well as a reactive element, in the aluminium alloy matrix
seems to fulfill all the above three requirements. The
important role played by the magnesium during the
composite synthesis is the scavenging of the oxygen
from the dispersoid surface, thus thinning the gas layer
and improving wetting action with the surface of the
dispersoids.As concluded from previous research
studies the strengthening of aluminium alloys with a
dispersion of fine particulates strongly increases their
potential in tribological and structural applications.
Rohatgi  reports that with the increase in volume
percentages of fly ash, hardness value increases in Al–
fly ash (precipitator type) composites. He also reports
that the tensile strength and elastic modulus of Al
composites increases with increase in volume
percentage (3–10%) of fly ash. Aghajanian and co
researchershave studied the Al2O3 particle reinforced
Al MMCs, improvement in elastic modulus, tensile
strength, compressive strength and fracture properties
with an increase in the reinforcement content. S. Sarkar,
S. Sen and S. C. Mishra  have studied on Al– fly ash
composite produced by impeller mixing and concluded
that up to 17wt% fly ash can be reinforced by liquid
metallurgy route and also the addition of magnesium
increases the wettability which leads mechanical
properties such as hardness, tensile strength and the
wear resistance. R.Q.Guo and P.K.Rohatgi  stated
that the slight decrease in density and strength of Al
composites with increasing weight per cent of fly ash
and the hardness increases slightly up to 10 wt % fly
ash, beyond with it decrease .
K. Radhakrishna and M. Ramachandra  have made
research on the effect of reinforcement of fly ash on
sliding wear, slurry erosive wear and corrosive behavior
of aluminium matrix composites produced by stir casting
method and concluded that Al (12 wt% Si) -15 wt% of fly
ash particulate composite improves the abrasive wear
moreover corrosion resistance
decreases as fly ash content increases.Sudarshan and
M.K.Surappa [22, 23] have synthesized A356 Al–fly ash
particle composites and studied on dry sliding wear
.They concluded that the addition of 6% of fly ash
particles into A356 Al alloy shows low wear rates at low
loads (10 and 20 N) while 12% of fly ash reinforced
composites show lower wear rates compared to the
unreinforced alloy in the load range 20–80 N.
The corrosion wear of composites is a critical design
criterion. D.M.Aylor and co researchers  stated that
pitting corrosion on Al-SiC composites was observed
predominantly at the interface between the Al and SiC.
Z.Feng and co researchers  analyzed the pitting
corrosion behaviour of Al-SiC 2024 composites and
attributed the corrosion of the composites to pit
formation at the Al-SiC interface.
P.K. Rohatgi, D.Weiss, and Gupta Nikhil  have
suggested that Al- fly composites can be used for
automotive and other applications due to their better
Al-fly ash composites offer many potential applications
particularly for internal combustion engine pistons and
Thus, much research has been carried out on particulate
metal matrix composites for tribological applications due
to the advantages of MMCs such as excellent wear
resistance, high load carrying capacity and light weight.
Though the aluminium alloys that restrict their
tribological behaviour, it has been approved by the
various researchers that increasing the ceramic
reinforcement particles content can improve the wear
Therefore, the application of aluminium matrix
composites is gradually increasing in the automotive
industries in making pistons, cylinder heads, connecting
rods etc. where the tribological properties of the material
are very important.
The wear resistance of particulate composites
significantly depends on the grit size, hardness, weight
fraction and distribution of reinforcement particles,
properties of matrix material, interfacial bonding between
the matrix and reinforcement particles and experimental
conditions such as hardness of the counter surface,
applied load, sliding distance and sliding speed.
Therefore, the present work aims to investigate
microstructure, mechanical, wear and corrosion
behaviour of fly ash particle reinforced commercial
aluminium composites fabricated by a two step stir
2.0 EXPERIMENTAL WORK
In this study, pure aluminium ingot with a purity of 99.5%
(weight fraction) was used as matrix material and fly ash
particle with average size of (50-100µm) were used as
the reinforcement materials and its chemical composition
was as shown in the table 1.
Table 1 Chemical composition of fly ash
54.27 34.73 6.1
In this research, Al - fly ash composites were produced
with a different amount of fly ash (ie 5, 10, 15, 20, 25 wt
%) by two step stir casting method. Stir casting setup is
shown in Fig.1
Figure.1 Stir casting setup
The fly ash particles were preheated to 600˙C for 2
hours in a separate muffle furnace to remove the
moisture content. Aluminium was charged in to the
graphite crucible, and the furnace temperature was
raised up to liquidus temperature 670˙C in order to melt
the Al scraps completely and further the melt
temperature was dropped to 620˙C attain the semi solid
state.1.5 wt% Magnesium and then preheated fly-ash
particles were added in the crucible. Mg was
incorporated into the melt to promote the wetting action
between Al matrix and fly ash reinforcement particles.
The molten Al composite slurry was stirred at the stirrer
speed of 300 rpm for 20 minutes. Since high torque was
needed in mixing of the composite slurry in semi solid
state, a variable torque - speed controlled mechanical
stirrer was employed. The dispersion of fly ash particles
with aluminium were achieved by the two step stirring
method. Finally the composite melt was reheated to
670˙C and poured into the steel mould to solidify.
Argon gas was blown at the rate of 2CC/min in to the
furnace during the process to prevent oxidation of
aluminium and magnesium. The melting was made in an
electrical resistive furnace (2Kw-1Kg capacity).
Temperatures were measured with a thermocouple (+/3 K error).
3.0 MICROSTRUCTURES ANALYSIS
Optic microscope and Scanning Electronic Microscope
(SEM) were employed to analyze the microstructure and
also the wear surface profile to decide the wear
mechanism of the material. Samples were mechanically
polished using sand metallographic practices and etched
with Keller’s regent prior to microstructure examination.
4.0 MECHANICAL PROPERTIES
Density of composites was obtained experimentally by
the Archimedian principle. Theoretical density was
calculated applying the rule of mixtures according to the
weight fraction of reinforcement.
Hardness test was performed on Al and composite
specimens. The hardness values of the specimen were
measured using Brinell hardness testing system with
10mm diameter at a load of 500 kg. The detention time
was 30 seconds. Three tests were taken on each
specimen to eliminate possibility of segregation and
mean value was considered.
Tensile and Compressive strength
Tensile and compressive strength tests were carried out
on Al specimens and composites using a computerized
UTM testing machine as per the ASTM E-8 standards.
Three samples were tested for each composition and
mean value was considered.
Normal loads: 5, 15 N.
Sliding speeds: 0.5, 1.0 m/s.
6.0 CORROSION WEAR
Corrosion is essentially an electrochemical process in
which an oxidation reaction occurs at the anode and a
reduction reaction occurs at the cathode.
The basic methodology is to measure the current flow in
the electrolyte medium, which is proportional to
corrosion rate with reference to potential applied. The
corrosion tests were conducted for the unreinforced Al
and composite specimens with varying weight % of fly
ash content (5%, 10%, 15%, 20% and 25%).
Al and Al – fly ash composite specimens were subjected
to corrosion test in 4% NaCl electrolyte solution at pH 3
using a standard Gill AC series-903 potentiostat.A
typical equipment consists of Applied Corrosion
electrochemical cell which consists of NaCl electrolyte, a
reference calomel electrode, a platinum auxiliary
electrode and a working electrode of the specimen.
The specimens were machined to the 20 mm dia and 20
mm length and were ground using 600grit emery paper,
rinsed in distilled water and methanol to remove surface
contaminants, and finally dried.
7.0 RESULTS AND DISCUSSION
Al - fly ash composites were successfully produced by a
two step stirring method which ensures homogenous
Figure.2 (a) Al – 10wt %fly ash Composites (stirring at
5.0 DRY SLIDING WEAR
A cylindrical pin of size 10mm diameter and 15mm
length (as shown in Fig.8) Al and composite specimens
were prepared and loaded in a computer interfaced pin
on disc wear testing rig. Before testing, the surface of
the specimens was abraded by using 1000 grit paper.
The rotating disc was made of EN 32 steel of diameter
75 mm and hardness of 65HRC. Wear tests were carried
out at room temperature for 20 minutes.
The test parameters are as follows:
Figure.2 (b) Al -10wt % fly ash Composites (stirring at
semi solid state)
Fig.2a) shows the SEM micrograph of Al-10wt% fly ash
composites fabricated by mechanical stirring duration of
20 minutes with the stirring speed of 300 rpm at 670 ˚C
(above liquidus) and Fig.2 (b) shows at 615˚C (in semi
It was observed from the Fig.2 (b) that fly ash particles
distribute homogeneously in the composites when the
stirring was made in semisolid condition. The
homogeneous distribution of fly ash particles in the Al
matrix was achieved due to smashing action of solid
dendrites in semi solid state. The interface between
matrix and reinforcement was almost perfectly bonded.
7.1 MECHANICAL BEHAVIOUR - The graph of
theoretical and experimental densities of the composites
according to the fly ash content is shown in Fig.3.
Generally the fly ash particles are having low density in
nature. In the present study precipitator type fly ash was
used which density is less than 2.2 g/cm .
The density of the composite specimens was determined
experimentally by the Archimedes principle. The small
pieces cut from the specimens were weighed first in air
and then water and density values were calculated using
the following expression.
of fly ash particles
Figure. 4 Hardness of the Composites at various Wt% of
fly ash particles
weight in air
(weight in air - weight in water)
Theoretical density values were determined using the
rule of mixtures relation.
The experimental density values of the Al-fly ash
composites decreased linearly with addition of fly ash
particles. The decrease in density of composites can be
attributed to lower density of fly ash particles than that of
the unreinforced Al.
It was also noted that the theoretical values closely
matches with the experimental values when the fly ash
content is less than 20 wt%. It indicates that the interface
between matrix and reinforcement was almost perfectly
bonded the prepared castings are dense and sound.
However when the fly ash content increases beyond
20wt%, there is a mismatch between the theoretical and
measured density values due to increased porosity and
Figure.5 Tensile strength of the Composites at various
Wt% of fly ash particles
Figure.6 Compressive strength of the Composites at
various Wt% of fly ash particles
Figure. 3 Density of the Composites at various Wt%
Table 2. Mechanical properties of Al and Al -fly ash
The results of the hardness test are given in the Table.2
which shows the values of hardness with the weight
fraction of fly ash.
As indicated in Fig.4, the increasing trend of hardness
was observed with increase in weight fraction of fly ash
particles up to 20%.Beyond this hardness trend started
decreasing. Incorporation of fly ash particles up to
20wt% significantly improves the hardness of the Al
matrix. The presence of fly ash particles in the
composites enhances the dislocation density which
resists the deformation when it is subjected to strain.
When the fly ash content increased from 5% to 20% by
weight, hardness increases from 25 BHN to 51 BHN.It
can be reasoned to the fact that the fly ash particles
possess higher hardness than the Al.
Tensile strength tests were performed and the results of
the test are shown in Fig.5.The results shows that the
tensile strength of composites is higher than that
obtained for the unreinforced Al. The tensile strength of
unreinforced Al is 77 MPa and this value increases to a
maximum of 113MPa for Al- 15 wt% fly ash composite
which is about 35% improvement on that of the
unreinforced Al matrix. When the fly ash content
increased from 20% to 25%, tensile strength decreases
from 113 MPa to 104 MPa.
It was observed that the composites containing more
than 15wt% of fly ash particles the rate of increase in
tensile strength decreases abruptly.
The results of the compression tests are showed in
Fig.6. The results revealed that the incorporation of fly
ash particles significantly improves the compressive
strength of Al matrix. However the compressive strength
of the composites begins to drop when the fly ash
content increased from 20 % to 25 wt%. Beyond 20 wt%,
the fly ash particles interact with each other due to
particles clustering which deteriorates the properties. It
may be noted that the composites subjected to
compressive stress, Al matrix around fly ash particles
flows away in the direction perpendicular to the applied
load which reduces the load transfer ability of the matrix.
It can be concluded that the mechanical properties such
as density, hardness, tensile and compressive strengths
of the composites increases by increasing fly ash
content. The addition of magnesium improves the
wettability between the fly ash particles and enhances
the mechanical properties of the composites by solid
solution strengthening. And also mechanical stirring in
the semi solid state enhances the uniform distribution
It was also observed from the Table.2 that the trend of
declining mechanical properties such as hardness,
tensile and compressive strengths of the composites
with increasing fly ash content beyond 15 – 20 wt%.
Agglomeration of fly ash particles could reduce the
interfacial bonding between Al and fly ash particles.
The diffusion of Mg at the Al- fly ash interface could also
result in Mg depletion from the matrix, accounting for the
reduction of the Mg2Si particle size which leads to a
decrease in solid solution strengthening. Hence results
in the decline in the mechanical properties of the
Figure .7 Few tested specimens (A: Wear; B: Tensile
strength; C: Hardness)
7.2 SLIDING WEAR BEHAVIOUR - The average
wear losses of the composites were examined as a
function of fly ash particle content at various load and
sliding speed conditions against carbon steel as
illustrated graphically in Figures. 8 and 9.Few tested
wear pin specimens are shown in Fig.7
Figure 8. Wear loss of Al specimen and Al –fly ash
composites as a function of sliding speeds 0.5 m/s and
1m/s at constant load 5N.
Figure 10. The worn surface of the Al – wt 5%fly ash
with a normal load of 5N with 1m/s Sliding velocity
Figure.9 wear loss of Al and Al –fly ash composites
specimen as a function of of sliding speeds 0.5 m/s and
1m/s at constant load 15N
Wear, the progressive loss of material
from the sliding surfaces of the elements of a tribosystem can be determined in terms of weight loss. The
material properties of the sliding elements, applied load
and sliding speed determine the wear rate. The wear
resistance of the Al- fly ash reinforced composites is
increased compared to the unreinforced Al at all sliding
speed and load conditions. The drastic decrease in wear
loss was observed with the incorporation of
The decreasing tendency of the wear rate of the
Al- fly ash composites was observed from the Fig.8
when the sliding speed increases from 0.5 m/s to 1m/s
at low load (5N) and lower concentration of fly ash (<20
wt %). It is obvious that the work hardening of the
aluminium occurs during the sliding action and also
formation of iron oxide film (Fe O ) on the surface of the
pin which enhances the wear resistance.
Fig.9 indicates that the wear rate of the Al
increased as the sliding speed increases and the same
trend of was observed in Al – fly ash composites at
higher load 15N
At higher speed (1m/s) and load (15 N)
conditions, the thermal softening effect of the Al lowers
the interfacial bond between the Al and fly ash materials
and also the protective oxide layer smashed out during
the sliding action resulting in higher wear loss . By
superimposing the Fig.8 and Fig.9, it can be observed
that the wear rate of the Al and Al- fly ash composites
increases as the load increases from 5 N to 15 N. The
obtained results are inline with the other researchers
Since the Al matrix is much softer than the
carbon steel disc, the steel might larger depth of
penetration into the surface and cut severely, causing
plastic deformation of the surface resulting in a great
amount of material loss. The worn surface of the Al – wt
5%fly ash has been described by little plastic
deformation as shown in Fig.10.
Further, from the Figures 8and 9, the trends of the wear
resistance can be found to be increased with increase of
fly ash content in the composites. This increase in wear
resistance of the composite may be due to the reason
the reinforcement material is much harder than that of
the matrix material.
The wear grooves and scratches along the sliding
direction were smaller due to the presence of fly ash
particulates. This shows that the presence of fly ash in
the matrix offers a resistance to wear.
Figure 11. The worn surface of the Al – wt25%fly ash
composite with a normal load of 15N with 0.5m/s Sliding
Applied load affects the wear behaviour of composites
and is the most dominating factor in controlling the wear
The worn surface of the Al composite with 25 wt% fly
ash was characterized by many pulling-out and
exposures of the fly ash particles and there were more
wear debris which indicated the poor interfacial strength
between the Al matrix and fly ash particles. Large
grooves and scratches appeared on the worn surfaces
as shown in Fig. 11 and there was no obvious indication
of plastic deformation.
The wear mechanism changed to abrasive wear from
The lowest wear loss was obtained for composite with
20wt% fly ash compared to composites reinforced with 5
wt %, 10 wt % and 15 wt % fly ash.Al-20wt% fly ash
composite demonstrated wear resistance approximately
7 times higher than that of unreinforced Al at 1 m/s
sliding speed and 5N load conditions. This is because
the fly ash particles have increased the hardness of Al
considerably as shown in Table 2 .This increase in wear
resistance can also be attributed to a better interfacial
bonding between Al and fly ash particles and thus helps
in preventing the damages caused due to sliding action.
The incorporation of only 20wt% fly ash particles
to the Al matrix was very effective to reduce its wear
loss. This is because of the interfacial bond which plays
a vital role in transferring loads from the Al matrix to the
hard fly ash particles. As the fly ash content increases
beyond 20 wt% the wear loss increased with increasing
the load. This may be due to clustering of fly ash
particles and poor interfacial bonding between Al matrix
and fly ash particles.
When the two surfaces are in sliding contact, wear
mechanisms such as surface abrasion, oxidation,
delamination and adhesion may happen either
separately or in combination.
The surface morphologies of the worn composites
indicate the following.
1.At low loads, fly ash particles support the load
and prevents Al matrix have direct contact with the
counter part thus helps in preventing the damages
caused due to sliding action. Abrasion wear mechanism
2. Higher applied load results in stresses which
exceed fracture stress of fly ash particles, these particles
loose their capacity to sustain the load. Also the hard fly
ash particles create scars on the surface of the steel
counter face which in turn causes higher wear rate of the
composite. The worn out particles also act as third body
abrasives initiate friction and could penetrate the
opposing surfaces in a contact zone which lead micro
ploughing action at its interface.
3. At lower sliding speeds abrasion is dominant,
while at higher sliding speeds delamination and
It follows from the above observations that the
main wear mechanism at higher loads and high sliding
speeds is delaminating wear causing excessive fracture
of the reinforcement and the matrix, resulting in
deterioration of the wear resistance of the composites.
When the composite is subjected to the higher
applied load with higher sliding speed, cracks on the
surface propagates in the subsurface which brings loss
of material from the worn surface in the form of flakes or
thin sheets. Also the considerable amount of Iron debris
transferred from the counter face to the composite pins.
Delamination was observed to be more
extensive under the higher load of 20N.
7.3 CORROSION WEAR BEHAVIOUR - The
corrosion wear of composites is influenced by several
factors such as porosity, high dislocation densities at the
matrix-reinforcement interfaces, the presence of
intermetallic compounds and interfacial reaction
products, and the electrical conductivity of the reinforcing
Corrosion wear was evaluated in terms of
mm/year for the fabricated Al and Al – fly ash
composites with varying proportion of fly ash content.
Electro chemical polarization reactivation curves
(EPR) were obtained with the help of ACM software.
Corrosion current and corrosion rate were determined
using the following expression specified by ASTM G190.
Corrosion rate in mm/year = [Icorr ×Metal factor]/1000
I corr =
(ba × bc)
, A / m2
[ 2.3 × Rp × (ba + bc)]
ba is anodic Tafel slope in Volts
bc is the cathodic Tafel slope in Volts
Rp is the polarization resistance in W/m
Metal factor = ( t × K ) / ρ
Where, t (seconds in year), ρ is the specimen density in
weight % of element × atomic weight of element
96487 × Valency of element
It can be observed from the EPR curve which is shown
in Fig.13 for Al-15wt% fly ash composite indicates a
decrease of the corrosion potential and an increase of
the corrosion current density than that of EPR curve of
Al which is shown in Fig.12. It may be noted that the
high corrosion density of Al- fly ash composites
increases the rate of Al dissolution due to pH variations
at the interface.
Figure 12 .EPR curve for Al
Figure 13.EPR curve for Al-15wt% fly ash composite
The results showed that the corrosion and pitting
potentials of Al were superior to Al- fly ash composites.
Figure.14 Corrosion wear of Al and Al- fly ash
Fig.14 shows that Al and Al- 25wt% fly ash composite
had the lowest and highest corrosion rate, respectively.
The corrosion rate of Al- 25wt%fly ash Composite is
increased about 10 times of the Al.
According to the general qualitative classification of
corrosion rates, moderate corrosion behaviour is seen
when the fly ash content is less than 15wt%.
The incorporation of fly ash to the Al matrix releases Ferich intermetallic phases such as Al3Fe / Al6Fe which
behaves as cathode. The occurrence of intermetallic
phase at the interface provide a platform for the electron
exchange needed for oxygen reduction and increases
the anodic reaction at a higher rate in the composites as
compared to an aluminium.Hence, the formation of
galvanic couples between the intermetallics and the Al
matrix causes dissolution of Al matrix and finally the
detachment of Al particles lead formation of pits. When
the fly ash content increases beyond 10wt%, corrosion
resistance of the composites is drastically increased
.This can be attributed to the formation of more
intermetallic clusters, porosities and voids at the
The Al –fly ash composites was successfully fabricated
by two step stir casting process in order to attain
homogenous distribution of fly ash particles in the Al
matrix. The distribution of fly ash particles was further
improved by the addition of 1.5 wt%Mg.
Based on the experimental observations the following
conclusions are drawn.
1. The density of the composites decreased with
increasing fly ash reinforcement content. Hence Al- fly
ash composites can be used in applications where
weight reductions are desirable.
2. Hardness, tensile strength and compressive strength
were determined for the test materials. Increasing fly ash
content resulted in increase in the tensile strength of the
Al. However, the tensile strength begins to drop when
the fly ash content exceeds 15wt% due to the decrease
in solid solution strengthening and particle clustering.
Hardness and compressive strength of composites
found increasing with increased fly ash content. Above
20 wt% of fly ash, both hardness and compressive
strength of composites begins to decrease.
3. The wear resistance of the commercial Al was
considerably enhanced by the addition of fly ash
particles and the wear resistance of the composites was
much superior to the unreinforced aluminium over the
entire load range tested under dry sliding conditions.
It may be due to the favorable effect of the fly ash
particles which is a dominating factor affecting the wear
resistance. However the addition of only 20wt% fly ash
particle to the Al was very effective to reduce its wear
4. It was observed that the high proportion of fly ash
reinforcement shows the poor resistance to corrosion.
Moderate corrosion resistance is seen when the fly ash
content is about 15 wt%
The results conclude that the Al-fly ash composites
could be considered as an excellent material in sectors
where light weight, enhanced mechanical properties and
wear resistance are prime consideration especially in
Kobashi, M. and Choh, T. (1993) ‘Wettability and
the Reaction for SiC Particle/Al Alloy System’,
Journal of Materials Science, Vol. 28.
Ahlatci, H. Karakas, M.S. Candan, E and
Cimenoglu, H. (2003) ‘Effect of Magnesium
Addition on Wear Behaviour of Al-70 Vol.-% Al2O3p
Composites’, Materials Science & Technology, Vol.
Liu, Y.L Kang, S.B. and Kim, H.W. (1999)
‘Complex Microstructures in As-Cast Al-Mg-Si
Alloy’, Materials Letters, Vol. 41.
Rohatgi, P.K. Kim, J.K. Guo, R.Q. Robertson, D. P.
and Gajdardziska-Josifovska, M. (2002) ‘Age
Hardening Characteristics of Aluminium Alloy –
Hollow Fly Ash Composites’, Metallurgical &
Materials Transaction A, Vol. 33A.
Rohatgi, P. K. and Guo, R. Q. (1997) ‘Low Cost
Cast Aluminium – Fly Ash Composites for Ultra
light Automotive Application’, TMS Annual
Meeting, Automotive Alloys.
Aghajanian, M. K. Langensiepen, R. A. Rocazella,
M. A. Leighton, J. T. Andersson, C. A. Mater, J. Sci.
28 (1993) 6683–6690
Golden, D. M. (1994) ‘Solidification Processing of
Metal Matrix Fly Ash Particle Composites’, EPRI
Rohatgi, P.K. Guo, R. Q. Iksan, H. Borchelt, E. J.
and Asthana, R. (1998) ‘Pressure Infiltration
Technique for Synthesis of Aluminium-Fly Ash
Particulate Composite’, Metallurgical & Materials
Transaction A, Vol. A244.
Guo, R. Q. and Rohatgi, P. K. (1998) ‘Chemical
Reactions Between Aluminium and Fly Ash During
Synthesis and Reheating of Aluminium-Fly Ash
Composite’, Metallurgical & Materials Transaction
B, Vol. 29B.
Lloyd, D. J. (1994) ‘Particle Reinforced Aluminium
and Magnesium Matrix Composites’, International
Materials Reviews, Vol. 39.
Sarkar, S. , Sen, S. and Mishra, S. C. (2008)
‘Aluminium – fly ash composite produced by
impeller mixing, Journal of reinforced plastics and
Rohatgi, P. K., Weiss, D. and Gupta Nikhil, (2006)
‘Applications of fly ash in synthesizing low-cost
mmcs for automotive and other applications’,JOM.
Guo, R. Q., Rohatgi, P. K., (1997) ‘Preparation of
Aluminium-Fly Ash Particulate Composite By
Powder Metallurgy Technique’, Journal Of Material
Science pp.3971- 3974.
Guo, R. Q., Venugopalan, D. and Rohatgi, P. K.
(1998) ‘Differential Thermal Analysis to Establish
the Stability of Aluminium-Fly Ash Composites
during Synthesis and Reheating’, Metallurgical &
Materials Transaction A, Vol. A241.
Guo, R. Q., Rohatgi, P. K. and Nath, D. (1996)
‘Compacting Characteristics of Aluminium-Fly Ash
Powder Mixtures’, Journal of Materials Science, Vol.
Rohatgi, P. K., Guo, R., Keshavaram, B. N. and
Golden, D. M. (1995) ‘Cast Aluminium,Fly Ash
Transactions of the American Foundrymen’s Society,
Kolukisa, S., Topuz, A. and Sagin, A. (2003) ‘The
Production and Properties of Fly Ash Containing
Aluminium Matrix Composite Materials’, Practical
Metallography, Vol. 40.
Zhang, X. F., Wang, D. J. and Xie, G. (2002)
‘Manufacturing of Aluminium/Fly Ash Composites
with Liquid Reactive Sintering Technology’, Acta
Metallurgica Sinica, Vol. 15.
18. Matsunaga, T., Kim, J. K., Hardcastle, S. and
Rohatgi, P. K. (2002)15.2004 ‘Crystallinity and
selected properties of fly ash particles’, Materials
Science and Engineering A325 Coal combustion
product (CCP) production and use survey, American
Coal Ash Association.
19. Rohatgi, P. K., Guo, R. Q., Iksan, H., Borchelt, E. J.
and Asthana, R. (1998) Mater. Sci. Eng. A244,22-30.
20. Rohatgi, P. K., Guo, R., Keshavaram, B. N. and
Golden, D. M. (1995) Trans. Am. Foundrymen’s Soc.
103, 575-579 .
21. Radhakrishna, K., Ramachandra, M., (2007) ‘Effect
of reinforcement of fly ash on sliding wear, slurry
erosive wear and corrosive behavior of aluminium
matrix composite’, Wear 262, pp.1450–1462.
22. Sudarshan, and Surappa, M. K., (2008) ‘Synthesis of
fly ash particle reinforced A356 Al composites and
their characterization’, Materials Science and
Engineering A 480, pp.117–124.
23. Sudarshan, Surappa, M. K. (2008) ‘Dry sliding wear
of fly ash particle reinforced A356 Al composites’,
Wear 265, pp.349–360.
24. Aylor D.M and Moran P.J.(1985) “Effect of
Reinforcement on the Pitting Behaviour of
Aluminium-Base Metal Matrix Composites”, Journal
of the Electrochemical Society, Vol. 321, No. 6, pp.
25. Feng .Z , Lin C, Lin J, and Luo J(1998) “Pitting
Behaviour of SiCp/2024 Al Metal Matrix
Composites,” Journal of Materials Science, Vol. 33,
26. Ferhat Gul, Mehmet Acilar, (2004) “Effect of the
reinforcement volume fraction on the dry sliding
wear behaviour of Al–10Si/SiCp composites
produced by vacuum infiltration technique”,
Composites Science and Technology 64 1959–1970.